Chem. Mater. 2001, 13, 4239-4246
Gold-Nanocluster-Doped Inorganic-Organic Hybrid Coatings on Polycarbonate and Isolation of Shaped Gold Microcrystals from the Coating Sol Goutam De* and Debtosh Kundu Sol-Gel Division, Central Glass and Ceramic Research Institute, 196, Raja S.C. Mullick Road, Jadavpur, Kolkata 700 032, India Received January 23, 2001. Revised Manuscript Received July 2, 2001
Au-nanocluster-doped inorganic-organic hybrid coatings on polycarbonate substrates were prepared for the application of abrasion-resistant colored coatings as well as nonlinear optical material. The Au-doped sol was prepared by incorporating HAuCl4·4H2O into a composite sol derived from 3-(glycidoxypropyl)trimethoxysilane, tetraethylorthosilicate, and 3-(methacryloxypropyl)trimethoxysilane via hydrolysis-condensation and epoxy polymerization reactions. When the coated substrates were exposed under UV light, three reactions occurred simultaneously: (i) reduction of Au ions into metallic Au nanoclusters, (ii) polymerization of methacrylate groups, and (iii) strengthening of the silica network. As a result, the UVcured coatings became reddish-purple and more abrasion-resistant than the polycarbonate substrate. UV-vis spectroscopy and TEM of the films showed a peak at 530 nm due to the surface plasmon resonance of Au nanoclusters and the presence of 8-10 nm spherical Au nanoclusters, respectively. XRD of the films also showed the characteristic peaks of metallic Au nanoclusters. The inorganic-organic hybrid network at the sol stage also acted as a new breeding medium for the generation of shaped (triangular, hexagonal, prismatic, etc.) Au microcrystals from the Au-doped sol without UV irradiation. Electron diffraction suggests that these were single crystals with a preferential growth along the Au (111) plane.
Introduction At the molecular level, inorganic-organic hybrid coatings show promising applications as hard and abrasion-resistant coatings on plastic substrates.1-6 In addition, hybrid materials are considered to be the nextgeneration composite materials having a wide variety of applications7-16 as, for example, mesoporous materi* Corresponding author. Fax: +91 33 4730957. E-mail: [email protected]
hotmail.com. (1) Nass, R.; Arpac, E.; Glaubitt, W.; Schmidt, H. J. Non-Cryst. Solids 1990, 121, 370. (b) Schmidt, H. J. Non-Cryst. Solids, 1994, 178, 302. (c) Wen, J.; Jordens, K.; Wilkes, G. L. Mater. Res. Soc. Symp. Proc. 1996, 435, 207. (d) Schmidt, H. K.; Geiter, E.; Mennig, M.; Krug, H.; Becker C.; Winkler, R.-P. J. Sol-Gel Sci. Technol. 1998, 13, 397. (e) Sepeur, S.; Kunze, N.; Werner, B.; Schmidt, H. In Coationgs on Glass; Pulker, H., Schmidt, H., Aegerter, M. A., Eds.; Proc. 2nd Int. Conf. On Coatings on Glass (Saarbruecken, Germany); 1998; pp 319-322. (2) Floch, H. G.; Belleville, P. F. J. Sol-Gel Sci. Technol. 1994, 1, 293. (3) (a) Etienne, P.; Sempere, R.; Phalippou, J. J. Sol-Gel Sci. Technol. 1994, 2, 171. (b) Etienne, P.; Denape, J.; Paris, J. Y.; Phalippou, J.; Sempere, R. J. Sol-Gel Sci. Technol. 1996, 6, 287. (4) (a) Betrabet, C.; Wikes, G. L. Am. Chem. Soc. Polym. Prep. 1992, 33, 286. (b) Wang, B.; Wikes, G. L. J. Macromol sci. Pure Appl. Chem. 1994, A31, 249. (5) Wold, C. R.; Soucek, M. D. J. Coat. Technol. 1998, 70, 43. (6) Del Monte, F.; Cheben, P.; Grover, C. P.; Mackenzie, J. D. J. Sol-Gel Sci. Technol. 1999, 15, 73. (7) Novak, B. M. Adv. Mater. 1993, 5, 422. (8) Judeinstein, P.; Sanchez, C. J. Mater. Chem. 1996, 6, 511. (9) Chujo, Y. Curr. Opin. Solid State Mater. Sci. 1996, 1, 806. (10) Sims, S. D.; Berkett, S. L.; Mann, S. Mater. Res. Soc. Symp. Proc. 1996, 431, 77. (11) Burkett, S. L.; Sims, S. D.; Mann, S. Chem. Commun. 1996, 1367. (12) Reetz, M. T.; Zonta, A.; Simpelkamp, J. Angrew Chem. Int. Ed. 1995, 34, 301. (13) Zevin, M.; Reisfeld, R. Opt. Mater. 1997, 8, 37.
als through surfactant templates,10,11 heterogeneous biocatalysts,12 optical waveguides,13 contact lens materials,14 and bioactive materials.15 3-(Glycidoxypropyl)trimethoxysilane (GLYMO) and 3-(methacryloxypropyl)trimethoxysilane (MEMO) have been largely used as precursors for inorganic-organic hybrid sol-gel materials.1,2,9,17 Both GLYMO and MEMO have the ability to form simultaneously an inorganic network, tSi-O-Sit, through hydrolysis and condensation reactions of the alkoxy groups and organic network, poly(ethylene oxide) and polymethacrylate, through the polymerization of epoxy and methacrylate groups, respectively. In this paper we report Au-nanocluster-incorporated, hard inorganic-organic coatings on transparent polycarbonate (PC) substrates.18 Here, “dual organic functionality” i.e., the epoxy units of GLYMO (heat sensitive) and the methacrylate units of MEMO (light sensitive), is utilized for the organic part of the coatings. The inorganic part constitutes with the “silica” from GLYMO (14) Philipp, G.; Schmidt, H. J. Non-Cryst. Solids 1984, 63, 283. (15) Yabuta, T.; Tsuru, K.; Hayakawa, S.; Ohtsuki, C.; Osaka, A. J. Sol-Gel Sci. and Technol. 2000, 19, 745. (16) Sanchez, C.; Lebeau, B.; Ribot, F.; In, M. J. Sol-Gel Sci. Technol. 2000, 19, 745. (17) Innocenzi, P.; Brusatin, G.; Guglielmi, M.; Bertani, R. Chem. Mater. 1999, 11, 1672. (18) The polycarbonate substrates have several unique properties, e.g., excellent clarity, complete UV cutoff, self-extinguishing, heat resistant up to 120 °C, can withstand 250 times greater impact than glass (i.e. virtually unbreakable), but they are not scratch resistant enough for practical applications such as transparent windows and optical lens.
10.1021/cm0100570 CCC: $20.00 © 2001 American Chemical Society Published on Web 10/09/2001
Chem. Mater., Vol. 13, No. 11, 2001
De and Kundu
ingly, we also report here for the first time the formation of Au microcrystals from Au-doped inorganic-organic hybrid sols. Experimental Section
and MEMO, as well as tetraethylorthosilicate (TEOS). Finally, Au nanoclusters are generated in the hybrid matrix, which make the coatings reddish purple in color, due to the surface plasmon resonance (SPR) of Au nanoclusters.19 These colored inorganic-organic hybrid abrasion-resistant coatings on PC are applicable to both indoor and outdoor decorative purposes. It is also known that the presence of nanoclusters in a dielectric matrix enhances the third-order electronic susceptibility, χ(3), of the host by several orders of magnitude.19,20 Such materials are particularly promising for optoelectronics, aiming to design all-optical switching devices. However, research on the Au-nanocluster-doped sol-gel coatings is mostly confined to glassy matrixes and glass substrates.19,20 Therefore, the Au-nanocluster-doped inorganic-organic hybrid coatings on PC developed in this work may also be useful as an alternative nonlinear optical material. It is widely known that shape-controlled Au microcrystals can be obtained from an aqueous solution of HAuCl421-24 either by reduction with a suitable reducing agent, e.g., sodium citrate,21 citric acid,21 sodium borohydride,22 and pyrrole,22 or UV light.23,24 The sodium borohydride and pyrrole reductions were employed for the synthesis of thiol-stabilized Au nanoparticles.22 It has also been found that the rodlike micelles of hexadecyltrimethylammonium chloride operates as a template for the preparation of spherical to needle-shaped gold crystals from HAuCl4 solution following a UV irradiation technique.23 In the present study, we found that gold microcrystals of different shapes were separated out from the coating sol during storage. Accord(19) Gonella, F.; Mazzoldi, P. Metal Nanocluster Composite Glasses. In Handbook of Nanostructured Materials and Nanotechnology; Nalwa, H. S., Ed.; Academic Press: San Diego, 2000; Vol. 4, pp 81-158. (20) (a) De, G.; Mattei, G.; Mazzoldi, P.; Sada, C.; Battaglin, G.; Quaranta, A. Chem. Mater. 2000, 12, 2157. (b) Fukumi, K.; Chayahara, A.; Kadono, K.; Sakaguchi, T.; Hirono, Y.; Miya, M.; Hayakawa, J.; Satou, M. Jpn. J. Appl. Phys. 1991, 30, L742. (c) Matsuoka, J.; Mizutani, R.; Kaneko, S.; Nasu, H.; Kamiya, K.; Kadono, K.; Sakaguchi, T.; Miya, M. J. Jpn. Ceram. Soc. 1993, 101, 105. (d) De, G.; Tapfer, L.; Catalano, M.; Battaglin, G.; Cacavale, F.; Gonella, F.; Mazzoldi, P.; Haglund, R. F., Jr. Appl. Phys. Lett. 1996, 68, 3820. (e) Kundu, D.; Honma, I.; Osawa, T.; Komiyama, H. J. Am. Ceram. Soc. 1994, 77, 1110. (21) (a) Turkevich, J.; Stevenson, P. C.; Hiller, J. J. Discuss. Faraday Soc. 1951, 11, 55. (b) Milligan, W. O.; Morriss, R. H. J. Am. Chem. Soc. 1964, 86, 3461. (22) (a) Selvan, S. T. Chem. Commun. 1998, 351. (b) Torigoe, K.; Esumi, K. J. Phys. Chem. B 1999, 203, 2862. (23) Esumi, K.; Matshuhisa, K.; Torigoe, K. Langmuir 1995, 11, 3285. (24) Y. Zhou, C. Y. Wang, Y. R. Zhu, and Z. Y. Chen, Chem. Mater. 1998, 11, 2310.
Preparation of Sols. GLYMO (60 mmol) and TEOS (35 mmol) were first cohydrolyzed in the presence of hydrochloric acid (0.185 mmol) and water (150 mmol). The above liquid mixture was stirred at room temperature (26 ( 1 °C) for 1 h. During this period, the initial heterogeneous liquid mixture transformed to a homogeneous sol. The sol was then refluxed for 2 h at 80.5 °C.25 This refluxed sol was then cooled to 26 ( 1 °C, and a 1:1 (by volume) methanol solution of MEMO (20 mmol) and water (50 mmol) mixture was added under stirring. Stirring was continued for 1 h and the solution was refluxed again for 1 h at 72.5 °C25 to obtain a composite GLYMOTEOS-MEMO sol. The molar ratio of GLYMO:TEOS:MEMO was 3:1.75:1. To this composite 1-methylimidazole (8 mmol; dissolved in 150 mmol methanol) was added as an epoxy polymerization initiators. The sol was then refluxed for 1 h at 68 °C25 to polymerize the epoxy groups. A faint yellowish sol resulted. Finally, methacrylate polymerization initiator, benzyl (0.027 mmol), was added, and the sol was aged at room temperature for 48 h. This sol is designated as GTM sol. The Au-doped coating sol (Au-GTM sol) was prepared by incorporating HAuCl4·4H2O (4.0 mmol; dissolved in 90-125 mmol of methanol) into the GTM sol under stirring. The stirring was continued for 2 h, and the resulting yellow sol was left undisturbed and sealed for 16 h prior to use as a coating sol. The composition with respect to the equivalent gold metal and silica in the sol was 3.4 mol % Au, 96.6 mol % SiO2. Preparation of Coatings. The coatings were prepared from the GTM and Au-GTM sols on 3 mm thick transparent PC substrates (Lexan, GE plastics).26 Prior to the coating deposition, the PC substrates were first cleaned with a neutral detergent, followed by rinsing with distilled water and 2-propanol, and finally, boiled in 2-propanol for 5 min. The coatings were prepared using the dipping technique (Dip-master 200, Chemat Corporation) with withdrawal velocities in the range of 2-20 cm/min. Similar coatings on pure silica glass and silicon wafers (both sides polished) were also prepared for the UV-visible and IR spectral studies, respectively. Curing of the Coatings. The coatings were first dried at 60 °C in an air oven and then cured 5-20 s photochemically using UV light (Hg vapor lamp through silica glass tube), followed by thermal curing at 100 °C for 1 h. The UV curing was done by passing the oven-dried coated samples through the silica tube (UV light enters the silica tube from the Hg vapor lamp) with a velocity of 2 cm/s, covering a distance of 10 cm. The UV light is focused in such a way that it covers only the 10 cm central part of the silica tube. In this way a UV exposure of 5 s can be obtained by a single operation. This step was repeated up to four times to increase the UV exposure time. Gold Microcrystals from the Coating Sols. When the Au-GTM coating sol was stored under closed conditions (at 25 °C in absence of the light) for about 3-5 days,27 precipitation of gold microcrystals was observed. The intensity of the yellow (25) All the precursors used here have boiling points much higher than 80.5 °C. However, the boiling temperature of this liquid mixture becomes 80.5 °C due to the generation of methanol and ethanol during the course of hydrolysis and condensation reactions of alkoxy (-OCH3 and -OC2H5) groups following the equation tSi-OCH3/OC2H5 + H2O f tSi-OH + CH3OH/C2H5OH. Further lowering of refluxing temperatures to 72.5 °C and 68 °C are due to the addition of extra methanol in the reaction mixture. (26) Polycarbonates are manufactured by the reaction of bisphenol A and phosgene or diphenyl carbonate. The average molecular weight of this material is between 22 000 and 32 000. For further details, see: Milby, R. V. Plastics Technology; McGraw-Hill: New York, 1973; pp 292-294. (27) We have used 90-125 mmol of methanol to dissolve 4 mmol of HAuCl4·4H2O. Use of less methanol (